#------------------------------------------------------------------------------
#$Date: 2016-02-13 14:50:18 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176428 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/60/7036070.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7036070
loop_
_publ_author_name
'Zhang, Xinyuan'
'Yao, Jiyong'
'Jiang, Xingxing'
'Fu, Ying'
'Lin, Zheshuai'
'Zhang, Guochun'
'Wu, Yicheng'
_publ_section_title
;
 K3LaTe2O9: a new alkali-rare earth tellurate with face-sharing TeO6
 octahedra.
;
_journal_issue                   35
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15576
_journal_page_last               15582
_journal_paper_doi               10.1039/c5dt02255j
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'K3 La O9 Te2'
_chemical_formula_weight         655.41
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-06-12 deposited with the CCDC.
2015-07-24 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   6.0589(9)
_cell_length_b                   6.0589(9)
_cell_length_c                   15.024(3)
_cell_measurement_reflns_used    1918
_cell_measurement_temperature    153.1500
_cell_measurement_theta_max      31.4147
_cell_measurement_theta_min      2.7115
_cell_volume                     477.64(14)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153.1500
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Rigaku AFC10 diffractometer'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0377
_diffrn_reflns_av_sigmaI/netI    0.0178
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            4437
_diffrn_reflns_theta_full        31.41
_diffrn_reflns_theta_max         31.41
_diffrn_reflns_theta_min         2.71
_exptl_absorpt_coefficient_mu    11.792
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6731
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    4.557
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Chip
_exptl_crystal_F_000             580
_exptl_crystal_size_max          0.1700
_exptl_crystal_size_mid          0.1450
_exptl_crystal_size_min          0.0900
_refine_diff_density_max         1.078
_refine_diff_density_min         -0.751
_refine_diff_density_rms         0.165
_refine_ls_extinction_coef       0.0246(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   2.135
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         344
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      2.135
_refine_ls_R_factor_all          0.0233
_refine_ls_R_factor_gt           0.0227
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0100P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0463
_refine_ls_wR_factor_ref         0.0465
_reflns_number_gt                340
_reflns_number_total             344
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt02255j1.cif
_cod_data_source_block           a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 7036070.cif.
;
_cod_original_sg_symbol_H-M      P63/mmc
_cod_database_code               7036070
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
K1 K 0.0000 0.0000 0.7500 0.0086(4) Uani 1 12 d S
K2 K 0.3333 0.6667 0.61656(11) 0.0122(3) Uani 1 6 d S
La1 La 0.0000 0.0000 0.5000 0.00297(16) Uani 1 12 d S
Te1 Te -0.3333 0.3333 0.65593(3) 0.00287(15) Uani 1 6 d S
O1 O -0.0592(7) 0.4704(4) 0.7500 0.0049(7) Uani 1 4 d S
O2 O -0.6412(5) 0.1794(2) 0.5945(2) 0.0088(6) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 K1 O2 143.43(4) 16_657 3_445
O2 K1 O2 65.84(8) 16_657 17_567
O2 K1 O2 143.43(4) 3_445 17_567
O2 K1 O2 143.43(4) 16_657 2_565
O2 K1 O2 65.84(8) 3_445 2_565
O2 K1 O2 102.27(10) 17_567 2_565
O2 K1 O2 65.84(9) 16_657 18_447
O2 K1 O2 102.27(11) 3_445 18_447
O2 K1 O2 65.84(8) 17_567 18_447
O2 K1 O2 143.43(4) 2_565 18_447
O2 K1 O2 102.27(11) 16_657 1_655
O2 K1 O2 65.84(8) 3_445 1_655
O2 K1 O2 143.43(4) 17_567 1_655
O2 K1 O2 65.84(8) 2_565 1_655
O2 K1 O2 143.43(4) 18_447 1_655
O2 K1 O1 120.57(5) 16_657 2
O2 K1 O1 55.07(5) 3_445 2
O2 K1 O1 93.67(5) 17_567 2
O2 K1 O1 93.67(5) 2_565 2
O2 K1 O1 55.07(5) 18_447 2
O2 K1 O1 120.57(5) 1_655 2
O2 K1 O1 55.07(5) 16_657 3
O2 K1 O1 93.67(4) 3_445 3
O2 K1 O1 120.57(5) 17_567 3
O2 K1 O1 120.57(5) 2_565 3
O2 K1 O1 93.67(4) 18_447 3
O2 K1 O1 55.07(5) 1_655 3
O1 K1 O1 120.0 2 3
O2 K1 O1 93.67(5) 16_657 .
O2 K1 O1 120.57(5) 3_445 .
O2 K1 O1 55.07(5) 17_567 .
O2 K1 O1 55.07(5) 2_565 .
O2 K1 O1 120.57(5) 18_447 .
O2 K1 O1 93.67(5) 1_655 .
O1 K1 O1 120.000(1) 2 .
O1 K1 O1 120.000(2) 3 .
O2 K1 O1 55.07(5) 16_657 2_665
O2 K1 O1 120.57(5) 3_445 2_665
O2 K1 O1 93.67(5) 17_567 2_665
O2 K1 O1 93.67(5) 2_565 2_665
O2 K1 O1 120.57(5) 18_447 2_665
O2 K1 O1 55.07(5) 1_655 2_665
O1 K1 O1 168.28(14) 2 2_665
O1 K1 O1 48.28(14) 3 2_665
O1 K1 O1 71.72(14) . 2_665
O2 K1 O1 93.67(4) 16_657 1_545
O2 K1 O1 55.07(5) 3_445 1_545
O2 K1 O1 120.57(5) 17_567 1_545
O2 K1 O1 120.57(5) 2_565 1_545
O2 K1 O1 55.07(5) 18_447 1_545
O2 K1 O1 93.67(4) 1_655 1_545
O1 K1 O1 48.28(14) 2 1_545
O1 K1 O1 71.72(14) 3 1_545
O1 K1 O1 168.28(14) . 1_545
O1 K1 O1 120.0 2_665 1_545
O2 K1 O1 120.57(5) 16_657 3_455
O2 K1 O1 93.67(5) 3_445 3_455
O2 K1 O1 55.07(5) 17_567 3_455
O2 K1 O1 55.07(5) 2_565 3_455
O2 K1 O1 93.67(5) 18_447 3_455
O2 K1 O1 120.57(5) 1_655 3_455
O1 K1 O1 71.72(14) 2 3_455
O1 K1 O1 168.28(14) 3 3_455
O1 K1 O1 48.28(14) . 3_455
O1 K1 O1 120.000(1) 2_665 3_455
O1 K1 O1 120.000(2) 1_545 3_455
O1 K2 O1 76.72(9) 3_565 .
O1 K2 O1 76.72(9) 3_565 2_665
O1 K2 O1 76.72(9) . 2_665
O1 K2 O2 96.15(6) 3_565 3_455
O1 K2 O2 56.20(7) . 3_455
O1 K2 O2 132.56(8) 2_665 3_455
O1 K2 O2 56.20(7) 3_565 1_665
O1 K2 O2 96.15(6) . 1_665
O1 K2 O2 132.56(8) 2_665 1_665
O2 K2 O2 64.62(10) 3_455 1_665
O1 K2 O2 132.56(8) 3_565 2_565
O1 K2 O2 56.20(7) . 2_565
O1 K2 O2 96.15(6) 2_665 2_565
O2 K2 O2 54.59(10) 3_455 2_565
O2 K2 O2 118.84(2) 1_665 2_565
O1 K2 O2 56.20(7) 3_565 2_675
O1 K2 O2 132.56(8) . 2_675
O1 K2 O2 96.15(6) 2_665 2_675
O2 K2 O2 118.84(2) 3_455 2_675
O2 K2 O2 54.59(10) 1_665 2_675
O2 K2 O2 166.55(12) 2_565 2_675
O1 K2 O2 132.56(8) 3_565 1_655
O1 K2 O2 96.15(6) . 1_655
O1 K2 O2 56.20(7) 2_665 1_655
O2 K2 O2 118.84(2) 3_455 1_655
O2 K2 O2 166.55(13) 1_665 1_655
O2 K2 O2 64.62(10) 2_565 1_655
O2 K2 O2 118.84(2) 2_675 1_655
O1 K2 O2 96.15(6) 3_565 3
O1 K2 O2 132.56(8) . 3
O1 K2 O2 56.20(7) 2_665 3
O2 K2 O2 166.55(12) 3_455 3
O2 K2 O2 118.84(2) 1_665 3
O2 K2 O2 118.84(2) 2_565 3
O2 K2 O2 64.62(10) 2_675 3
O2 K2 O2 54.59(10) 1_655 3
O1 K2 Te1 34.63(5) 3_565 1_665
O1 K2 Te1 103.71(4) . 1_665
O1 K2 Te1 103.71(4) 2_665 1_665
O2 K2 Te1 93.52(5) 3_455 1_665
O2 K2 Te1 31.62(5) 1_665 1_665
O2 K2 Te1 147.62(5) 2_565 1_665
O2 K2 Te1 31.62(5) 2_675 1_665
O2 K2 Te1 147.62(5) 1_655 1_665
O2 K2 Te1 93.52(5) 3 1_665
O1 K2 Te1 103.71(4) 3_565 .
O1 K2 Te1 34.63(5) . .
O1 K2 Te1 103.71(4) 2_665 .
O2 K2 Te1 31.62(5) 3_455 .
O2 K2 Te1 93.52(5) 1_665 .
O2 K2 Te1 31.62(5) 2_565 .
O2 K2 Te1 147.62(5) 2_675 .
O2 K2 Te1 93.52(5) 1_655 .
O2 K2 Te1 147.62(5) 3 .
Te1 K2 Te1 117.278(16) 1_665 .
O1 K2 Te1 103.71(4) 3_565 1_655
O1 K2 Te1 103.71(4) . 1_655
O1 K2 Te1 34.63(5) 2_665 1_655
O2 K2 Te1 147.62(5) 3_455 1_655
O2 K2 Te1 147.62(5) 1_665 1_655
O2 K2 Te1 93.52(5) 2_565 1_655
O2 K2 Te1 93.52(5) 2_675 1_655
O2 K2 Te1 31.62(5) 1_655 1_655
O2 K2 Te1 31.62(5) 3 1_655
Te1 K2 Te1 117.278(16) 1_665 1_655
Te1 K2 Te1 117.278(16) . 1_655
O2 La1 O2 180.0 13_456 1_655
O2 La1 O2 87.49(10) 13_456 14_546
O2 La1 O2 92.51(10) 1_655 14_546
O2 La1 O2 92.51(10) 13_456 2_565
O2 La1 O2 87.49(10) 1_655 2_565
O2 La1 O2 180.00(12) 14_546 2_565
O2 La1 O2 87.49(10) 13_456 15_666
O2 La1 O2 92.51(10) 1_655 15_666
O2 La1 O2 87.49(10) 14_546 15_666
O2 La1 O2 92.51(10) 2_565 15_666
O2 La1 O2 92.51(10) 13_456 3_445
O2 La1 O2 87.49(10) 1_655 3_445
O2 La1 O2 92.51(10) 14_546 3_445
O2 La1 O2 87.49(10) 2_565 3_445
O2 La1 O2 180.00(10) 15_666 3_445
O2 La1 K1 52.98(7) 13_456 13_556
O2 La1 K1 127.02(7) 1_655 13_556
O2 La1 K1 52.98(7) 14_546 13_556
O2 La1 K1 127.02(7) 2_565 13_556
O2 La1 K1 52.98(7) 15_666 13_556
O2 La1 K1 127.02(7) 3_445 13_556
O2 La1 K1 127.02(7) 13_456 .
O2 La1 K1 52.98(7) 1_655 .
O2 La1 K1 127.02(7) 14_546 .
O2 La1 K1 52.98(7) 2_565 .
O2 La1 K1 127.02(7) 15_666 .
O2 La1 K1 52.98(7) 3_445 .
K1 La1 K1 180.0 13_556 .
O2 La1 K2 128.793(14) 13_456 1_545
O2 La1 K2 51.207(14) 1_655 1_545
O2 La1 K2 63.61(7) 14_546 1_545
O2 La1 K2 116.39(7) 2_565 1_545
O2 La1 K2 128.793(14) 15_666 1_545
O2 La1 K2 51.207(14) 3_445 1_545
K1 La1 K2 116.59(2) 13_556 1_545
K1 La1 K2 63.41(2) . 1_545
O2 La1 K2 51.207(14) 13_456 13_566
O2 La1 K2 128.793(14) 1_655 13_566
O2 La1 K2 116.39(7) 14_546 13_566
O2 La1 K2 63.61(7) 2_565 13_566
O2 La1 K2 51.207(14) 15_666 13_566
O2 La1 K2 128.793(14) 3_445 13_566
K1 La1 K2 63.41(2) 13_556 13_566
K1 La1 K2 116.59(2) . 13_566
K2 La1 K2 180.00(4) 1_545 13_566
O2 La1 K2 128.793(14) 13_456 .
O2 La1 K2 51.207(14) 1_655 .
O2 La1 K2 128.793(14) 14_546 .
O2 La1 K2 51.207(14) 2_565 .
O2 La1 K2 63.61(8) 15_666 .
O2 La1 K2 116.39(8) 3_445 .
K1 La1 K2 116.59(2) 13_556 .
K1 La1 K2 63.41(2) . .
K2 La1 K2 101.50(3) 1_545 .
K2 La1 K2 78.50(3) 13_566 .
O2 La1 K2 51.207(14) 13_456 13_556
O2 La1 K2 128.793(14) 1_655 13_556
O2 La1 K2 51.207(14) 14_546 13_556
O2 La1 K2 128.793(14) 2_565 13_556
O2 La1 K2 116.39(8) 15_666 13_556
O2 La1 K2 63.61(8) 3_445 13_556
K1 La1 K2 63.41(2) 13_556 13_556
K1 La1 K2 116.59(2) . 13_556
K2 La1 K2 78.50(3) 1_545 13_556
K2 La1 K2 101.50(3) 13_566 13_556
K2 La1 K2 180.0 . 13_556
O2 Te1 O2 97.52(12) 2_565 .
O2 Te1 O2 97.52(12) 2_565 3_455
O2 Te1 O2 97.52(12) . 3_455
O2 Te1 O1 92.18(9) 2_565 .
O2 Te1 O1 165.24(12) . .
O2 Te1 O1 92.18(9) 3_455 .
O2 Te1 O1 92.18(9) 2_565 3_455
O2 Te1 O1 92.18(9) . 3_455
O2 Te1 O1 165.24(12) 3_455 3_455
O1 Te1 O1 76.29(12) . 3_455
O2 Te1 O1 165.24(11) 2_565 2_565
O2 Te1 O1 92.18(9) . 2_565
O2 Te1 O1 92.18(9) 3_455 2_565
O1 Te1 O1 76.29(12) . 2_565
O1 Te1 O1 76.29(12) 3_455 2_565
O2 Te1 Te1 119.74(9) 2_565 16_557
O2 Te1 Te1 119.74(9) . 16_557
O2 Te1 Te1 119.74(9) 3_455 16_557
O1 Te1 Te1 45.50(8) . 16_557
O1 Te1 Te1 45.50(8) 3_455 16_557
O1 Te1 Te1 45.50(8) 2_565 16_557
O2 Te1 K2 59.284(17) 2_565 1_445
O2 Te1 K2 59.284(17) . 1_445
O2 Te1 K2 140.67(10) 3_455 1_445
O1 Te1 K2 117.94(3) . 1_445
O1 Te1 K2 54.10(8) 3_455 1_445
O1 Te1 K2 117.94(3) 2_565 1_445
Te1 Te1 K2 99.60(3) 16_557 1_445
O2 Te1 K2 59.284(17) 2_565 .
O2 Te1 K2 140.67(10) . .
O2 Te1 K2 59.284(17) 3_455 .
O1 Te1 K2 54.10(8) . .
O1 Te1 K2 117.94(3) 3_455 .
O1 Te1 K2 117.94(3) 2_565 .
Te1 Te1 K2 99.60(3) 16_557 .
K2 Te1 K2 117.278(16) 1_445 .
O2 Te1 K2 140.67(10) 2_565 1_455
O2 Te1 K2 59.284(17) . 1_455
O2 Te1 K2 59.284(17) 3_455 1_455
O1 Te1 K2 117.94(3) . 1_455
O1 Te1 K2 117.94(3) 3_455 1_455
O1 Te1 K2 54.10(8) 2_565 1_455
Te1 Te1 K2 99.60(3) 16_557 1_455
K2 Te1 K2 117.278(16) 1_445 1_455
K2 Te1 K2 117.278(16) . 1_455
O2 Te1 K1 51.74(9) 2_565 .
O2 Te1 K1 126.04(5) . .
O2 Te1 K1 126.04(5) 3_455 .
O1 Te1 K1 53.614(7) . .
O1 Te1 K1 53.614(7) 3_455 .
O1 Te1 K1 113.50(8) 2_565 .
Te1 Te1 K1 68.000(7) 16_557 .
K2 Te1 K1 66.756(14) 1_445 .
K2 Te1 K1 66.756(14) . .
K2 Te1 K1 167.60(3) 1_455 .
O2 Te1 K1 126.04(1) 2_565 1_565
O2 Te1 K1 126.04(1) . 1_565
O2 Te1 K1 51.74(9) 3_455 1_565
O1 Te1 K1 53.614(6) . 1_565
O1 Te1 K1 113.50(8) 3_455 1_565
O1 Te1 K1 53.614(7) 2_565 1_565
Te1 Te1 K1 68.000(7) 16_557 1_565
K2 Te1 K1 167.60(3) 1_445 1_565
K2 Te1 K1 66.756(14) . 1_565
K2 Te1 K1 66.756(14) 1_455 1_565
K1 Te1 K1 106.828(8) . 1_565
Te1 O1 Te1 89.00(15) . 16_557
Te1 O1 K2 179.72(12) . 16_557
Te1 O1 K2 91.28(4) 16_557 16_557
Te1 O1 K2 91.28(4) . .
Te1 O1 K2 179.72(15) 16_557 .
K2 O1 K2 88.45(11) 16_557 .
Te1 O1 K1 94.18(4) . .
Te1 O1 K1 94.18(4) 16_557 .
K2 O1 K1 85.80(5) 16_557 .
K2 O1 K1 85.80(5) . .
Te1 O1 K1 94.18(4) . 1_565
Te1 O1 K1 94.18(4) 16_557 1_565
K2 O1 K1 85.80(5) 16_557 1_565
K2 O1 K1 85.80(5) . 1_565
K1 O1 K1 168.28(14) . 1_565
Te1 O2 La1 172.71(16) . 1_455
Te1 O2 K1 99.13(12) . 1_455
La1 O2 K1 88.15(8) 1_455 1_455
Te1 O2 K2 89.10(5) . 1_445
La1 O2 K2 91.74(5) 1_455 1_445
K1 O2 K2 83.57(6) 1_455 1_445
Te1 O2 K2 89.10(5) . 1_455
La1 O2 K2 91.74(5) 1_455 1_455
K1 O2 K2 83.57(6) 1_455 1_455
K2 O2 K2 166.55(12) 1_445 1_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
K1 O2 3.000(3) 16_657
K1 O2 3.000(3) 3_445
K1 O2 3.000(3) 17_567
K1 O2 3.000(3) 2_565
K1 O2 3.000(3) 18_447
K1 O2 3.000(3) 1_655
K1 O1 3.0505(18) 2
K1 O1 3.045(5) 3
K1 O1 3.045(5) .
K1 O1 3.045(5) 2_665
K1 O1 3.045(5) 1_545
K1 O1 3.045(5) 3_455
K2 O1 2.875(3) 3_565
K2 O1 2.875(3) .
K2 O1 2.875(3) 2_665
K2 O2 3.051(4) 3_455
K2 O2 3.051(4) 1_665
K2 O2 3.051(4) 2_565
K2 O2 3.051(4) 2_675
K2 O2 3.051(4) 1_655
K2 O2 3.0505(18) 3
K2 Te1 3.5478(6) 1_665
K2 Te1 3.5478(6) .
K2 Te1 3.5478(6) 1_655
La1 O2 2.358(3) 13_456
La1 O2 2.358(3) 1_655
La1 O2 2.358(3) 14_546
La1 O2 2.358(3) 2_565
La1 O2 2.358(3) 15_666
La1 O2 2.358(3) 3_445
La1 K1 3.7560(8) 13_556
La1 K2 3.9119(9) 1_545
La1 K2 3.9119(9) 13_566
La1 K2 3.9119(9) 13_556
Te1 O2 1.860(3) 2_565
Te1 O2 1.860(3) .
Te1 O2 1.860(3) 3_455
Te1 O1 2.016(3) .
Te1 O1 2.016(3) 3_455
Te1 O1 2.016(3) 2_565
Te1 Te1 2.8267(10) 16_557
Te1 K2 3.5478(6) 1_445
Te1 K2 3.5478(6) 1_455
Te1 K1 3.7728(5) 1_565
O1 Te1 2.016(3) 16_557
O1 K2 2.875(3) 16_557
O1 K1 3.045(5) 1_565
O2 La1 2.358(3) 1_455
O2 K1 3.000(3) 1_455
O2 K2 3.0505(18) 1_445
O2 K2 3.0505(18) 1_455
